## Thermoelectric Materials

Thesis by

Alexandra Zevalkink

In Partial Fulfillment of the Requirements for the Degree of

Doctor of Philosophy

California Institute of Technology Pasadena, California

2013

ii

© 2013 Alexandra Zevalkink

Acknowledgments

First and foremost, I would like to thank my husband, Alex, for supporting me and putting up with me throughout my time as a graduate student. All of my family members have been extremely supportive and encouraging, for which I am immensely grateful.

None of this work would have been possible without the advice and guidance of my research adviser, Jeff Snyder, who has been an absolute pleasure to work with for the past five years.

I have also benefited from the help of several close collaborators who have con-tributed to this work both intellectually and experimentally. Eric Toberer is responsi-ble for starting me down the path of Zintl research, and guiding the first several years of work on the materials in this thesis. Greg Pomrehn performed the majority of the computational work, and Wolfgang Zeier contributed his considerable knowledge of solid state chemistry.

iv

## Abstract

Zintl phases, a subset of intermetallic compounds characterized by covalently-bonded “sub-structures,” surrounded by highly electropositive cations, exhibit precisely the characteristics desired for thermoelectric applications. The requirement that Zintl compounds satisfy the valence of anions through the formation of covalent substruc-tures leads to many unique, complex crystal strucsubstruc-tures. Such complexity often leads to exceptionally low lattice thermal conductivity due to the containment of heat in low velocity optical modes in the phonon dispersion. To date, excellent thermoelectric properties have been demonstrated in several Zintl compounds. However, compared with the large number of known Zintl phases, very few have been investigated as thermoelectric materials.

From this pool of uninvestigated compounds, we selected a class of Zintl anti-monides that share a common structural motif: anionic moieties resembling infinite chains of linked MSb4 tetrahedra, where M is a triel element. The compounds

were found to have filled valence bands and exhibit intrinsic electronic properties.
Doping with divalent transition metals (Zn2+ _{and Mn}2+_{) on the}_{M}3+ _{site, or Na}1+_{on}
the A2+ _{site allowed for rational control of the carrier concentration and a transition}
towards degenerate semiconducting behavior. In optimally-doped samples, promising
peakzT values between 0.4 and 0.9 were obtained, highlighting the value of continued

vi

## Contents

Acknowledgments iii

Abstract iv

List of Figures ix

List of Tables xxv

1 Introduction 1

1.1 Thermoelectric Energy Conversion . . . 1

1.2 Introduction to Zintl Phases . . . 3

1.2.1 Zintl Chemistry . . . 3

1.2.2 Thermoelectric Zintl Phases . . . 6

1.3 Electronic Transport in Zintl phases . . . 7

1.3.1 Carrier Concentration Optimization . . . 7

1.3.2 Band Structure Criteria . . . 11

1.3.3 Carrier Relaxation Time . . . 13

1.4 Lattice Thermal Conductivity . . . 14

1.4.1 Introduction . . . 14

1.4.2 Thermal Conductivity within the Debye Model . . . 16

1.4.3 Thermal Conductivity in Complex Systems . . . 20

1.5 Summary of Research . . . 26

2.2 Characterization . . . 31

2.3 Analysis of Transport Properties . . . 34

2.4 Density Functional Theory . . . 35

3 Thermoelectric Properties of Ca5M2Sb6 (M = Al, Ga, or In) 37 3.1 Introduction . . . 37

3.2 Influence of the Triel Elements (M = Al, Ga, In) on the Properties of Ca5M2Sb6 . . . 39

3.3 Optimization of Ca5Al2Sb6 . . . 53

3.3.1 Na-doped Ca5Al2Sb6 . . . 53

3.3.2 Zn-doped Ca5Al2Sb6 . . . 62

3.3.3 Mn-doped Ca5Al2Sb6 . . . 69

3.4 Optimization of Ca5Ga2Sb6 via Zn doping . . . 77

3.5 Optimization of Ca5In2Sb6 via Zn doping . . . 85

4 Thermoelectric Properties of Sr5Al2Sb6 95 4.1 Introduction . . . 95

4.2 Results and Discussion . . . 96

4.3 Conclusion . . . 100

5 Thermoelectric Properties of Ca3AlSb3 103 5.1 Introduction . . . 103

5.2 Na-doped Ca3AlSb3 . . . 104

5.3 Zn-doped Ca3AlSb3 . . . 119

6 Thermoelectric properties of Sr3GaSb3 127 6.1 Introduction . . . 127

6.2 Results and Discussion . . . 130

6.3 Conclusion . . . 137

viii

7.2 Results and Discussion . . . 141

7.3 Conclusion . . . 147

8 Comparison of A5M2Sb6 and A3MSb3 Zintl Compounds 149 8.1 Electronic Structure . . . 149

8.2 Electronic Transport Properties . . . 152

8.3 Thermal Transport Properties . . . 154

8.4 Figure of Merit . . . 156

A List of A5M2Pn6 and A3MPn3 Compounds 159

A Lattice thermal conductivity of Zintl antimonides 161

## List of Figures

1.1 a) Schematic of a thermoelectric generator. b) A balance between insu-lating and metallic behavior must be achieved to obtain high zT. . . . 2

1.2 Examples of classic Zintl structure types with 0-, 2-, and 3-dimensional anionic substructures. . . 5

1.3 Influence of Zn doping on the room temperature (a) carrier concentra-tion, (b) Seebeck coefficient and conductivity, and (c-d) figure of merit of Ca5In2Sb6. . . 8

1.4 Left panel: The carrier concentration in Yb14Al1−xMnxSb11 increases

linearly with increasingx. Right panel: In contrast, in Ca5Al2−xMnxSb6,

n increases linearly only at very low Mn concentrations. . . 9

1.5 (a)AZn2Sb2samples (A= Sr, Eu, Ca, Yb) have a broad range of carrier

concentrations, but all can be described by the same band mass (m∗ =

0.6 me) within a single parabolic band model. (b) In contrast, the

mobility of AZn2Sb2 samples varies widely, suggesting large differences

in the carrier relaxation time, τe. . . 13

1.6 Thermoelectric materials can achieve low lattice thermal conductivity through point scattering sources (Si1−xGex, XyCo4Sb12 [1, 2, 3]), heavy

x

1.7 In a Debye model, the speed of sound (νs), phase velocity (νp), and

group velocity (νg) are equivalent. In contrast, the Born-von Karman

model for a monoatomic chain shows significant curvature of the phonon dispersion. . . 16

1.8 (a) Spectral Debye heat capacity approaches ω2 dependence at high temperatures. (b) Frequency dependence of common scattering mecha-nisms. (c) Top curve: spectral thermal conductivity (assuming νg(ω) =

νs and T >> θD) when τU limits transport. Lower curve: spectral

thermal conductivity when τB, and τP D are also accounted for. . . 18

1.9 Calculated κU (Eq. 1.11) significantly overestimates experimentalκL in

rock salt compounds with high mass contrast atT =θD. Values for θD,

γ and κL were obtained from Ref. [7] . . . 21

1.10 (a) As mass contrast increases in a diatomic chain, (average mass, νs

held constant) the optical mode flattens and the gap increases. (b) The reduction of κL due to mass contrast can be judged from the area

beneath the νg(ω)2 curves. . . 21

1.11 For materials with many atoms per primitive cell (N), Eq. 1.11 fails to predict the experimental κL. Data obtained from ref [8]. . . 23

1.12 (a) Phonon dispersions for ball and spring chains with increasing number of atoms per unit cell (constant νs). (b) A dramatic decrease in νg(ω)2,

and thus κs(ω), is found with increasing N. For N = 4 and 8, the

high frequency optical modes are not visible on a linear plot due to the extreme flatness of these modes. . . 24

1.13 Success of κa+κo in predicting the lattice thermal conductivity of

se-lected materials (see supplementary Table 1). Here, κa includes both

3.1 (a) The orthorhombic unit cell of Ca5Al2Sb6 (P bam) viewed down the

[001] direction. (b) Adjacent tetrahedral chains, oriented along the [001] axis, are connected by Sb-Sb bonds. Sb atoms are orange, Ca are green, and Al are blue. . . 37

3.2 (a) Electron density difference isosurfaces show regions of charge accu-mulation in a Ca5Al2Sb6 unit cell, and (b) along the AlSb4 tetrahedral chains. Al atoms are blue, Sb in orange, and Ca in green. . . 40

3.3 (a-c) The conduction band minima of Ca5M2Sb6 (M=Al, Ga, In)

com-pounds contain discreet anti-bonding states corresponding to Sb-Sb (1) and M-Sb (2) interactions. The position of the M-Sb anti-bonding

peak influences Eg. (d-f) The band structures reveal a high degree of

anisotropy. The lightest band mass (m∗

X−U) is parallel to the anionic

“ladders”, while the perpendicular directions (m∗

X−S and m∗X−Γ) are far

heavier. . . 41

3.4 XRD patterns of polished, polycrystalline Ca5M2Sb6(M = Ga, In)

sam-ples (colored curves) and Rietveld fits using the known crystal structures (black curves) [9]. The reflections belonging to CaSb2 are indicated by red asterisks. . . 44

3.5 Optical absorption measurements at room temperature reveal direct band gaps in the Ca5M2Sb6 samples, with the band gap in the Ga ana-logue (0.43 eV) significantly smaller than the Al or In anaana-logues (0.65 eV and 0.64 eV, respectively). . . 45

3.6 The temperature dependence of (a) the resistivity and (b) the Hall car-rier concentration of Ca5M2Sb6 samples is indicative of intrinsic

semi-conducting behavior. (c) Hall mobility at 300 K is highest in the Ga-analogue, consistent with its lower band mass. (d) Seebeck coefficients decrease with temperature due to activation of minority carriers. Band gaps estimated from Eg ∝ 2αmaxTmax are consistent with results from

xii

3.7 The band gap, Eg, is determined from ρ ∝ eEg/2kBT, where ρ is the

resistivity in the intrinsic temperature regime. . . 47 3.8 The thermal conductivity in Ca5M2Sb6 (M = Al, Ga, In) is dominated

by the lattice term at room temperature and by the bipolar term at higher temperatures. Ca5In2Sb6 exhibits the lowest κL due to its

rela-tively dense, soft lattice. . . 51 3.9 Scanning electron micrographs of (a) a polished surface and (b) a

frac-ture surface of Ca4.75Na0.25Al2Sb6 following hot pressing. . . 54

3.10 Powder XRD patterns for Ca5−xNaxAl2Sb6 (x = 0, 0.5), Rietveld fit to

the Ca5Al2Sb6 structure and difference profile for thex = 0 pattern. . 55

3.11 (a) Na levels in Ca5−xNaxAl2Sb6 track the synthetic composition well

(dashed line) up to a maximum ofx=0.25. (b) Hall effect measurements

show that n increases with Na content at less than the predicted rate

(dashed line), and does not exceed 2×1020 _{h}+ _{cm}−3_{. . . .} _{56}
3.12 (a-b) The resistivity of Ca5−xNaxAl2Sb6decreases with increasingx. (c)

The Hall carrier concentration is relatively constant with temperature for all compositions. (d) Samples with low doping levels show some evidence for activated behavior leading to a positive slope in the mobility near room temperature. The decay in mobility at higher temperatures is associated with phonon scattering. . . 57 3.13 Carrier concentration (n) dependence of room temperature Seebeck

co-efficients compared to a single parabolic band model with an effective mass of 2.2 me. . . 58

3.14 High temperature Seebeck coefficients of Ca5−xNaxAl2Sb6show

decreas-ing magnitude with increasdecreas-ing Na dopdecreas-ing. . . 58 3.15 (a) The total thermal conductivity and (b) the lattice component for

Ca5−xNaxAl2Sb6. The minimum thermal conductivity is obtained from

Eq. 3.8. By assessing the optical mode contribution to the minimum thermal conductivity (κmin optical), the experimental acoustic

3.16 (a)The high temperature thermoelectric figure of merit (zT) of Ca5−xNaxAl2Sb6

samples increases with increasing temperature. ExperimentalzT versus

carrier concentration at 700K. (b) The optimization of zT with carrier

concentration was confirmed using a single parabolic band model with parameters given in the text. . . 61

3.17 Ca5Al2−xZnxSb6 X-ray diffraction patterns (x= 0,0.20), Rietveld fit to

the x= 0sample and associated difference profile. No secondary phases

are observed for the x range investigated (0< x <0.20). . . 63

3.18 With zinc doping, the carrier concentration at 300 K is directly propor-tional to the level predicted using simple electron counting (dashed line). This is in contrast to the lower doping efficiency with sodium [10]. . . . 64

3.19 (a) The Hall carrier concentration of Ca5Al2−xZnxSb6 samples increases

withx. Doped samples exhibit extrinsic behavior to 800 K. (b) Undoped

Ca5Al2Sb6 exhibits a mobility dominated by phonon scattering across the entire temperature range investigated, while Zn-doped samples show evidence of additional scattering mechanisms at low temperature. (c) High temperature resistivity and (d) Seebeck coefficients decrease with increasing Zn doping level, and show degenerate behavior for the extrin-sically doped compositions, similar to the Na-doped analog [10]. . . 65

3.20 Similar Seebeck coefficient values for Na- and Zn-doped Ca5Al2Sb6 at equivalent carrier concentrations suggest similar band mass. Curve gen-erated using a single parabolic band approximation and an effective mass of 1.8 me [10]. . . 66

3.21 (a) Total thermal conductivity of Ca5Al2−xZnxSb6 increases with

in-creasing doping level and thus electronic conductivity. (b) The lattice contribution (κL) decays with T−1 and approaches a minimum value at

high temperature, consistent with prior Na-doped compositions [10]. To calculate κL, Lorenz coefficients (inset) were calculated using the single

xiv

3.22 Compared to sodium-doped Ca5Al2Sb6, the reduced mobility of the sam-ples in this study lead to lower zT. Within the Zn series, the highest

doped composition exhibits the largest zT. . . 68

3.23 SEM images of fracture surfaces of (a)x= 0.1 and (b) x= 0.3 samples,

hot pressed a total of 7 and 9 hours, yielding grain sizes of 1-10µm and >10µm, respectively. (c) Backscatter electron image of a polished

sur-face (x=0.4) showing representative phase fractions of Ca5Al2−xMnxSb6

(light grey), Ca11Sb10 (dark grey), and CaSb2 (white). . . 70

3.24 XRD patterns of polished polycrystalline samples of Ca5Al2−xMnxSb6

(x= 0.05, 0.1, 0.2, and 0.3) and Rietveld fit using the known Ca5Al2Sb6

structure. In most samples (x=0.05, 0.2, 0.3) peaks from minority

phases Ca11Sb10 and CaSb2 are also present. . . 71

3.25 With substitution of the larger Mn2+ ions on the Al3+ site, the unit cell of Ca5Al2Sb6 expands in the direction parallel to tetrahedral chains (c)

and contracts in the direction perpendicular to both chains and Sb-Sb bonds (b). . . 72

3.26 Room temperature Hall carrier concentrations increase with dopant con-centration for Mn-, Zn-, and Na-doped Ca5Al2Sb6. In practice, Na and Mn are not fully activated dopants relative to the predicted relationship assuming one free hole per dopant atom (solid line). . . 73

3.28 Experimental Seebeck coefficients at 300 and 700 K of Mn-, Zn-, and Na-doped Ca5Al2Sb6. Solid curves were generated using a single parabolic band model with an effective mass of 1.8 me and 2.0 me for 300 K and

700 K, respectively. . . 75

3.29 (a) Total thermal conductivity and (b) lattice thermal conductivity of Ca5Al2−xMnxSb6 (x = 0.05, 0.1, 0.2, 0.3) and Ca5−xNaxAl2Sb6 (x =

0.25) samples. The inset shows the temperature dependence of the
Lorenz numbers in units of 108 W_{Ω}_{K}−2, calculated using a single
para-bolic band model. . . 76

3.30 The figure of merit of Ca5Al2−xMnxSb6 samples remains below that of

Ca5−xNaxAl2Sb6 within the measured temperature range. . . 77

3.31 XRD patterns of Ca5Ga2−xZnxSb6 (x = 0 and x = 0.3) are shown in

black. A small amount of the secondary phase CaSb2 was observed in all samples. In the sample with x = 0, the asterisk denotes a reflection

from CaSb2. The simulated Rietveld fits are overlaid in red, and the difference profile is shown in red underneath. . . 78

3.32 (a) The Hall carrier concentration,nH, increases with increased Zn

con-tent, x. Inset: nH begins to deviate from the expected values shown by

the dashed line above x=0.2. (b) Resistivity decreases with increasing nH, showing a transition from intrinsic semiconducting to metallic

be-havior. (c) Hall mobility decreases with increasing x, but is improved

relative the Al-analogue, Ca5Al1.9Zn0.1Sb6. (d) The Seebeck coefficient decreases in magnitude and exhibits an increasingly linear temperature dependence with increasing Zn. . . 80

3.33 The experimental Seebeck coefficients of Ca5Ga2−xZnxSb6 at T = 300

and 500 K are compared with a single parabolic band model, show-ing general agreement. An effective mass of 1.6 me was used for both

xvi

3.34 (a) The total and (b) lattice thermal conductivity in Ca5Ga2−xZnxSb6.

The inset shows the Lorenz numbers, calculated from the SPB model using experimental Seebeck coefficients. . . 84

3.35 The figure of merit of Ca5Ga2−xZnxSb6 reaches a maximum of ∼0.35

at 750 K for samples with x = 0.05 and x = 0.1. The magnitude and

temperature of the peakzT are reduced relative to the Al analogue due

to the smaller band gap in Ca5Ga2Sb6. . . 85

3.36 XRD pattern of a polycrystalline slice of the x = 0.05 sample, Rietveld

fit using the known Ca5In2Sb6 structure, and difference profile. . . 86

3.37 (a) Backscattered electron image of a polished surface of Ca5In1.9Zn0.1Sb6 showing representative fractions of Ca5In2Sb6 (grey), a secondary phase (light grey), and pores (black). (b) Secondary electron image of a frac-ture surface of the same sample reveals grain sizes on the order of 1

µm. . . 87

3.38 With increasing Zn content, the Hall carrier concentration at 300 K in Ca5In2−xZnxSb6 increases as predicted by simple charge counting

(dashed line) up to x = 0.05 . . . 88

3.39 (a) With increasing x in Ca5In2−xZnxSb6, the carrier concentration

in-creases and (b) the resistivity dein-creases by an order of magnitude. (c) The Hall mobility decreases with Zn content, becoming comparable to Na-doped Ca5Al2Sb6 at high temperatures. (d) High temperature See-beck coefficients of Ca5In2−xZnxSb6 samples display increasingly linear

behavior and decreased magnitude with increased Zn concentration. . . 89

3.40 The Seebeck coefficients decrease as a function of n as predicted by a

single parabolic band model (solid curves). Effective masses of 2.0 me

(at 300 K and 500 K) and 1.8 me (at 700 K) were calculated from the

3.41 (a) The total thermal conductivity and (b) the combined lattice and bipolar thermal conductivity of Ca5In2−xZnxSb6. The inset shows the

temperature dependence of the Lorenz numbers in units of 108 _{W}_{Ω}_{K}−2_{,}
calculated using an SPB model. . . 91

3.42 The figure of merit of Ca5In2−xZnxSb6 samples is comparable to

Na-doped Ca5Al2Sb6 within the measured temperature range. . . 93

3.43 The figure of merit at 700 K is optimized at 2×1020 _{h}+_{cm}−3_{, in }
agree-ment with the SPB model. The parameters used at 300, 500, and 700 K,
respectively were m∗ = 2.0, 2.0, 1.8 me, κL = 1.2, 0.9, and 0.7 W/mK,

and intrinsic mobilities of 7.6, 6.9, and 5.3 cm2_{/Vs. . . .} _{94}

4.1 (a) The orthorhombic crystal structure of Sr5Al2Sb6(space groupPnma) is characterized by infinite anionic chains aligned in [100] direction. (b) Each chain is formed from alternately corner- and edge-sharing AlSb4 tetrahedra [11]. Sr atoms are shown in green, Sb in orange, and Al in blue. . . 96

4.2 The density of states of Sr5Al2Sb6 reveals a fully filled valence band and a relatively large band gap of 0.8 eV. . . 97

4.3 Rietveld analysis of the X-ray diffraction data for hot-pressed Sr5Al2Sb6 suggests that the samples are phase pure with no significant impurities. 98

4.4 (a) The resistivity decreases with temperature, confirming that Sr5Al2Sb6 is an intrinsic semiconductor. (b) The carrier concentration increases with temperature due to minority carrier activation, while the mobil-ity decreases due to acoustic phonon scattering. (c) The high, positive Seebeck coefficient is consistent with low, p-type nH. (d) The thermal

xviii

5.1 (a) The orthorhombic structure of Ca3AlSb3(Space group Pnma) viewed in the [010] direction. (b) Infinite chains of corner-sharing AlSb4 tetra-hedra extend in the [010] direction. Sb atoms are orange, Ca are green, and Al are blue. . . 104

5.2 (a) XRD pattern of x= 0 sample and Rietveld fit using known crystal

structures of Ca3AlSb3 and Ca5Al2Sb6 [12, 13]. (b) Similar amounts of Ca5Al2Sb6 impurity phase are observed in all sodium-doped samples . 105

5.3 Scanning electron micrographs of a) polished and b) fractured surfaces of the x= 0.06 sample reveal high density material and approximately

1 µm diameter grains. Black dots in (a) are voids revealed by polishing. 106

5.4 Microprobe analysis suggests that some sodium loss occurs during syn-thesis, and that the solubility limit of sodium in Ca3−xNaxAlSb3 is

ex-ceeded for x > 0.06 (0.8 atomic %). Filled symbols indicate Na content

of the matrix phases (Ca3AlSb3 and Ca5Al2Sb6), while unfilled symbols represent total Na concentration, including the Na-rich impurity phase. 107

5.5 Hall carrier concentration (300 K) increases as a function of sodium content, although doping effectiveness is less than predicted by charge counting. . . 108

5.6 (a) Hall carrier concentration of Ca3−xNaxAlSb3 as a function of

tem-perature. (b) Temperature dependence of the Hall mobility suggests an activated mobility at low temperature, and a mobility limited by phonon scattering at high temperature. (c) The resistivity as a function of temperature for x = 0.03, 0.06, 0.15. Inset: Ln[ρ] versus 1/T for x

= 0 sample. The high temperature linear fit results in a band gap of 0.6 eV. (d) The high temperature Seebeck coefficients show degenerate behavior for the extrinsically doped, p-type compositions. . . 109

5.7 Experimental Seebeck coefficients of Ca3−xNaxAlSb3 as a function of

5.8 Top panel: Calculated band structure of Ca3AlSb3. Bottom panel: Mag-nified band structure at the top of the valence band. The highest carrier concentration obtained experimentally corresponds to ∼0.1 eV below the valence band edge. The blue, yellow, and green dashed curves are parabolas with effective masses of 0.15, 0.75, and 0.9 me. . . 111

5.9 (a) EDD line-scans show charge accumulation and depletion along a chain-forming Al-Sb bond (green), and two distinct Al-Sb bonds per-pendicular to the chains (blue and orange). (b) Representative Ca-Sb bonds (site designations correspond to ref. [12]. . . 112 5.10 EDD isosurfaces show (a) accumulation and (b) depletion regions. (c)

Electron density map of valence band edge (-0.1 eV). Images are projec-tions along [010] (left side) and [201] (right side) direcprojec-tions. . . 113 5.11 Density of states of Ca3AlSb3 reveals a band gap at the Fermi level with

a valence band edge dominated by Sb p states. The inset highlights

interacting Al-Sb bonding states. . . 114 5.12 (a) Total thermal conductivity of Ca3−xNaxAlSb3 (x= 0, 0.03, 0.06,

0.15). (b) κL exhibits 1/T temperature dependence (dashed red curve).

At high temperatures, κL + κB approaches the glassy limit (dashed

black curve). The inset illustrates the temperature dependence of the
Lorenz numbers in units of 108 _{W}_{Ω}_{K}−2_{. . . 116}
5.13 (a) High temperature figure of merit of Ca3−xNaxAlSb3 yields a

max-imum value of 0.8 at 1050 K. (b) Experimental zT versus carrier

con-centration for Ca3−xNaxAlSb3. The dashed line was generated using

a single parabolic band model, with an effective mass of 0.8 me, and

intrinsic mobility 15 cm2_{/Vs and lattice thermal conductivity of 0.78}
W/mK. . . 117
5.14 X-ray diffraction data for Ca3Al1−xZnxSb3 including profile fit, profile

xx

5.15 Temperature dependence of the electrical resistivity, ρ, the Hall

car-rier concentration, nH, the Hall mobility, µH, and the Seebeck

co-efficient, α, of Ca3Al1−xZnxSb3. Experimental data is compared to

Ca2.94Na0.06AlSb3 data (black line).[5] . . . 121

5.16 Total thermal conductivity (top) and lattice thermal conductivity (bot-tom) of Ca3Al1−xZnxSb3. The inset illustrates the smaller grains (left)

for the compositions with x= 0.00, 0.02, and 0.05 and larger grain sizes

for x = 0.01 (right). . . 123

5.17 Experimental Seebeck coefficients as a function of carrier concentration (left) and figure of merit zT with temperature of Ca3Al1−xZnxSb3. . . 124

6.1 (a) Sr3GaSb3 contains unique chains of corner-sharing GaSb4tetrahedra, formed from four-tetrahedra repeat units. Ga atoms are green, Sb are orange, and Sr atoms are not shown. (b) The structure of Sr3GaSb3 viewed down the [101] axis, with chains going into the page (Sr atoms shown in blue). In both views, a single chain is highlighted in red. . . . 128

6.2 Top: back-scattered electron image of a polished Sr3GaSb3 sample re-veals the secondary phase Sr2Sb3 as white specks, while secondary elec-tron imaging of a fracture surface shows the very small grain size (<

1µm). Bottom: X-ray diffraction data for Sr3Ga1−xZnxSb3, including

profile fit, profile difference, and profile residuals from the correspond-ing Pawley refinement, includcorrespond-ing the secondary phase Sr2Sb3. Inset: the reflections indexed to the impurity phase are marked by asterisks. . . . 129

6.4 The temperature dependence of (a) the electrical resistivity, ρ, and (b)

the Hall carrier concentration, nH, in Sr3Ga1−xZnxSb3 illustrates the

transition towards degenerate semiconducting behavior upon Zn doping. (c) The Hall mobility,µH, reveals activated behavior at low temperature

and (d) the Seebeck coefficient,α, becomes more metallic with increasing

Zn. . . 134

6.5 (a) Total thermal conductivity and (b) lattice thermal conductivity of Sr3Ga1−xZnxSb3. The calculated minimum lattice thermal conductivity

κmin is shown as a broken line, and the inset shows the calculated Lorenz

numbers generated using an SPB model [6]. . . 135

6.6 (a) Seebeck coefficients (diamonds) and zT (circles) vary with carrier

concentration approximately according to an SPB model at 700 K. The solid and broken curves represent the predicted SPB behavior of α and zT, respectively, assuming m∗ = 0.9me, µ0 = 17 cm2V−1s−1 and κL =

0.55 Wm−1_{K}−1_{. (b) The measured figure of merit of Sr3}_{Ga1}

−xZnxSb3

exceeds 0.9 when heavily doped. . . 137

7.1 (a) The orthorhombic crystal structure of Sr3AlSb3 (space groupCmca) contains 56 atoms per primitive cell [14]. Sr atoms are shown in green, Sb in orange, and Al in blue. (b) Each isolated anionic moieties is made up of two edge-sharing tetrahedra (for clarity, Sr is not shown) [14]. . . 140

7.2 (top) Calculated site-projected density of states and (bottom) electronic band structure along the primary axes. The inset shows the 1st Brillouin zone with the k-points corresponding to each primary axis labeled. . . 141

xxii

7.4 (a)The resistivity and (b) carrier concentration of undoped and nomi-nally Zn-doped Sr3AlSb3 are indicative of intrinsic semiconducting be-havior. A band gap of Eg = 0.7 eV was estimated from the nominally

Zn-doped sample (see inset) (c) The Hall mobility of the undoped sample is comparable to that of Yb14MnSb11, and is increased by the addition of Zn. (d) The Seebeck coefficients are high, peaking at intermediate temperatures. . . 144

7.5 The thermal conductivity (κ) of Sr3AlSb3approaches the predicted

min-imum lattice thermal conductivity (κmin) at high temperature, due in

part to the complex unit cell. . . 145

7.6 An SPB model at 600 K (dashed line) assuming m∗=3 me and µo=2.8

cm2/Vs illustrates the potential improvement in _{zT} expected to result
from successful doping of Sr3AlSb3. . . 146

8.1 Dependence of the experimental Hall carrier concentration on dopant concentration. Dashed lines show the predicted carrier concentration as upper and lower bounds. . . 152

8.2 (a) The Hall mobility and (b) Seebeck coefficients of chain-forming Zintl compounds are a function of effective mass. . . 153

8.3 The room temperature lattice thermal conductivity of Zintl antimonides decreases with increasing unit cell volume. A5M2Sb6 andA3MSb3 com-pounds fit the expected trend. Data is tabulated in Appendix A. . . . 154

8.4 The speed of sound decreases with increasing density. The predicted decrease assuming constant shear and bulk moduli is illustrated by the dashed lines. . . 155

8.6 The figures of merit of optimally doped Ca3AlSb3 and Sr3GaSb3 and Ca5M2Sb6 samples highlight the importance of low κL and high

## List of Tables

1.1 Room temperature κL in materials with a large number of atoms (N)

per primitive cell. . . 22

2.1 The purity (% metals basis) and geometry of the elemental precursors are given below. Except for Ca dendrites from Sigma-Aldrich, all ele-ments were sourced from Alfa-Aesar. . . 30

2.2 Hot pressing parameters. . . 31

3.1 Given below for each compound is the electronegativity (χ), band gap

from mBJ calculations (Eg theor.), from optical absorption (Eg opt.),

and from resistivity (Eg ρ), the band mass, m∗, in three principle

direc-tions, and the estimated density of states effective mass, m∗

DOS. . . 42

3.2 Here, d is the theoretical density,Dis thermal diffusivity at 325 K, and κmin is the minimum lattice thermal conductivity at high temperature

(T >ΘD). . . 50

3.3 For Ca5In2Sb6 and Ca5Al2Sb6,d is theoretical density,D is thermal

dif-fusivity at 325 K and κmin is the minimum lattice thermal conductivity

at high temperature (T >ΘD) . . . 92

xxvi

8.2 Nv,edgeis the valence band degeneracy atEF=0, andNv,addis the number

of additional bands within 0.1 eV of the band edge. The single band
effective mass, m∗, is given in three perpendicular directions, where m∗_{1}

is parallel to the tetrahedral chains or pairs. m∗_{DOS} is the estimated

range for the density of states effective mass. . . 151 8.3 The number of atoms per unit cell (N), theoretical density (d), shear

and bulk moduli (G and K), and longitudinal and transverse speeds of

sound (νl and νt). . . 155

A.1 . . . 160

A.1 Room temperature lattice thermal conductivity,κL, for Zintl antimonides

## Chapter 1

Introduction

1.1

Thermoelectric Energy Conversion

Solving society’s current energy dilemma requires both broadening our energy re-sources and reducing our energy consumption. Since more than 50% of the energy consumed nationwide is lost as waste heat, the recovery of even a small fraction of this energy through the use of thermoelectric generators has the potential to significantly impact the global energy landscape [15]. While this solid state technology is currently used in extraterrestrial and other specialized applications, further improvements in cost and efficiency of thermoelectric materials are required for thermoelectric gener-ators to be competitive in most automotive and industrial waste heat applications.

The construction of a thermoelectric generator is shown schematically in Figure 1.1 a. Here, two thermoelectric ‘legs’ made of n-type and p-type materials are

alter-nated such that they are electrically in series and thermally in parallel. For power generation, the legs are placed across a temperature gradient, causing the carriers to move towards the cold end, and generating a voltage across each leg. This behavior, known as the Seebeck effect, is the basis of thermoelectric energy conversion. In re-verse, the same device operates as a Peltier cooler, where an applied voltage generates a temperature gradient [16].

2

Hot Side

Cold Side

e- _{h}+

e-

e-

e-

h+

h+

h+

a) b)

Figure 1.1: a) Schematic of a thermoelectric generator. b) A balance between insu-lating and metallic behavior must be achieved to obtain high zT.

coefficient (α) is the voltage generated due to a temperature gradient (α=∆V/∆T).

The electrical resistivity (ρ = 1/σ, where σ is conductivity) and thermal

conduc-tivity (κ), are, respectively, parasitic sources of voltage and heat loss, and must be

minimized. Traditional thermoelectric materials havezT near unity, corresponding to

about 10% of the Carnot efficiency. However there have been an increasing number of reports of largerzT through enhancements in both electronic and thermal properties

[19, 20, 21, 6].

Figure 1.1b illustrates the balance that must be achieved in order to obtain high thermoelectric efficiency; a large Seebeck coefficient is found in low carrier concen-tration (n) insulators, while high electrical conductivity is found in high carrier

con-centration metals. As a consequence, most good thermoelectric materials are heavily doped semiconductors with carrier concentrations between 1019 to 1021 carriers/cm3 [18]. Thermoelectric optimization is complicated by the transport of heat, which is carried by both phonons, which lead to lattice thermal conductivity (κL), and by

charge carriers, which lead to electronic thermal conductivity (κe) and bipolar

ther-mal conductivity (κB). The electronic term is related to the electrical conductivity

through the Wiedemann-Franz law (κe = LσT), where the Lorenz factor (L) can be

Ideal thermoelectric materials must therefore be both excellent electronic conduc-tors and poor phonon conducconduc-tors. This combination of properties is challenging to obtain due to the strongly coupled nature of α, ρ, and κ [18]. In the past decade,

however, several effective approaches have emerged for the design of such materials. One frequent strategy is the addition of phonon scattering sources, such as grain boundaries, impurities, or nano-precipitates, to reduce lattice thermal conductivity while minimally impacting charge carrier transport. This has been most successful in traditional semiconductors with inherently high electronic mobility such as Si [22]. A second promising approach is the manipulation of electronic band structures via either doping or alloying to take advantage of multiple charge carrier pockets in the Fermi surface. This leads to excellent thermoelectric properties in compounds such as LaTe and PbTe [19, 23]. Lastly, materials with complex crystal structures have been exploited for their inherently low lattice thermal conductivities. For example, ex-ceptionally low lattice thermal conductivity is found in the Zintl phase Yb14MnSb11, which contains 104 atoms in its primitive cell [21]. Such complexity results in glass-like lattice thermal conductivity at high temperatures, due to confinement of heat in low velocity, optical phonon modes, as well as additional opportunities for scattering events. This thesis, which describes the characterization and optimization of a new class of complex Zintl phases, favors the latter of these strategies.

1.2

## Introduction to Zintl Phases

1.2.1

Zintl Chemistry

4

that he developed to explain the formation of such structures were later extended and generalized by W. Klemm [27]. R. Hoffman has described the Zintl-Klemm concept as “the single most important theoretical concept in solid-state chemistry of the last century.” [28]

Chemically, Zintl phases can be placed between insulating, salt-like compounds
and intermetallic compounds [29]. In salt-like compounds (e.g., sulfates, phosphates,
and a vast array of silicates), both the anions and cations obtain a full octet or “18
electron shell.” Barite (BaSO4) is an excellent example, in which Ba donates its two
valence electrons to support the formation of [SO4]2− _{tetrahedra. Such compounds}

possess large band gaps, and generally exhibit insulating behavior. In contrast, many intermetallic phases, despite their highly complex, ordered structures, are electron deficient or lack a band gap, leading to metallic behavior.

Zintl phases are characterized by highly electronegative cations that donate their electrons to an anionic substructures. The Zintl-Klemm concept rationalizes the structural and bonding characteristics of Zintl phases by assuming that the cation transfers its valence electrons fully to the anions. The anions must in turn form covalently-bonded polyanions to obtain closed shells (filled octet) [24]. Referred to by W. Pearson as “valence compounds,” [30], Zintl phases are distinguished from other intermetallic compounds by their valence-precise nature. Fundamentally, Zintl phases are more closely related to the salt-like compounds described above, in which all octets are filled. However, the constituent elements in Zintl compounds are different, leading, ultimately, to different structure types and semiconducting rather than insulating electronic behavior. Zintls compounds are formed traditionally from a combination of an alkali or alkaline earth metal and a post-transition metal or metalloid from group 13, 14, 15, or 16. A classic example is NaSi, in which the Si atoms form [Si4]4−

The guiding principle for rationalizing the number of covalent bonds in a Zintl structure is given by the 8-N rule, in which N is the total valence electron count.

The total valence electron count (V EC) simply describes the total number of electrons

available to each anion in the structure, including those donated by the cations. For a binary compound, AaXx, the V EC is given by Eq. 1.1, where e(A) and e(X) are

the valence counts for A and X respectively. Typically, it is assumed that there are

no bonds between A atoms, and that X can have X−X bonds that are considered

to be two-center, two-electron bonds, and also that the octet rule is satisfied for both elements.

V EC = (a·e(A) +x·e(X))/x (1.1)

For example, in NaTl, V EC = (1·1 + 1·3) / 1 = 4. Since (8 - VEC) = 4, each Tl is expected to form four Tl-Tl bond. The resulting anionic structure is a Tl diamond lattice (B32, Strukturbericht classification). In NaSi, V EC = 5, requiring

the formation of 3 additional bonds per Si atom, and leading to the isolated [Si4]4−

tetrahedra observed in this structure type.

*A*Zn_{2}Sb_{2} (*A*=Ca, Sr, Eu, Yb)

Ca14AlSb11 CaAl2Si2 Ca3Al2Ge3

Figure 1.2: Examples of classic Zintl structure types with 0-, 2-, and 3-dimensional anionic substructures.

differ-6

ent types of anionic moieties. Take for example the extremely complex structure of
Ca14AlSb11, shown below in Figure 1.2a. A single formula unit contains 4 isolated
Sb3−_{, an [AlSb4]}9− _{tetrahedra, and a linear [Sb3]}7− _{moiety. The 14 Ca}2+ _{cations}
lead to overall charge-balance [34]. In many Zintl phases, extended 2-dimensional or
3-dimensional networks are formed. For example, in compounds with the CaAl2Si2
structure type (Figure 1.2b), Ca contributes two electrons to Al and Si, which form
infinitely extending 2-dimensional [Al2Si2]2−_{slabs [33]. Ca3}_{Al2Ge3, in contrast, forms}

a 3-dimensional net of corner-linked AlGe4 tetrahedra. [35]. The electron deficiency
of the [Al2Ge3]6− _{sublattice is balanced by the 3 Ca}2+ _{cations that reside in the }
tun-nels. In each case, the structure can be rationalized by using simple electron counting
rules. A testament to its effectiveness, the Zintl-Klemm concept is still used today to
guide the discovery of new structure types and compounds.

1.2.2

## Thermoelectric Zintl Phases

The rich chemistry of Zintl compounds leads to many of the characteristics desired for thermoelectric applications: complex structures, extensive opportunities to tune transport properties, narrow band gaps, and thermal and chemical stability [36, 37]. However, it was not until 2005 that Zintl compounds were recognized as potential thermoelectric materials with the discovery of highzT in Yb1−xCaxZn2Sb2 by Gascoin

et al.[32]. Shortly thereafter, the thermoelectric properties of the degenerately p

-doped Zintl compound Yb14MnSb11 were investigated by Brown et al in 2006 [38]. Yb14MnSb11 was found to have a figure of merit of 1 at 1000 K. Compared with the state-of-the-art high temperaturep-type material Si0.8Ge0.2, this was an improvement

arises from a small or negative band gap, there is very little potential for thermo-electric applications. Several recently discovered Zintl phases are known to possess band gaps, but the transport properties have not yet been fully characterized. For ex-ample, BaGa2Sb2, Ba4In8Sb16, Eu11Zn6Sb12, Eu7Ga6Sb8, Eu10Mn6Sb13, Ba2Sn3Sb6, Ba3Ga4Sb5, and Ba2In5As5 exhibit unique, complex structures and appear to have energy gaps in their electronic structures [49, 50, 51, 52, 53, 54, 55, 56]. However, the vast majority of known Zintl compounds have not been studied beyond the initial crystallographic characterization.

Clathrate compounds, characterized by covalent, anionic cages containing ionically-bonded cations, can also be considered Zintl phases [6]. Clathrate compounds have been the focus of frequent studies of their unique chemistry [57, 58] and excellent thermoelectric properties [59]. As they comprise their own field of study, they will not be discussed further here. Skutterudite compounds are yet another group of ex-cellent thermoelectric materials [60, 61, 62] that sometimes meet the definition of a Zintl phase, but are ubiquitous enough to be considered as a separate field of study.

1.3

## Electronic Transport in Zintl phases

1.3.1

Carrier Concentration Optimization

Due to their valence-precise nature, Zintl compounds are ideally semiconductors with
fully filled valence bands [36, 37], provided the band gap is greater than zero. Zintl
compounds generally behave as intrinsic semiconductors with very low carrier
con-centrations (n >1019 carriers/cm3), low electronic conductivity,_{σ}, and high Seebeck
coefficients,α. In contrast, high zT generally occurs in heavily doped semiconductors

with n between 1019-1020 carriers/cm3. Fortunately, most Zintl compounds can be doped to obtain degenerate semiconducting behavior, and by rationally optimizing the electronic properties, large improvements in zT relative to undoped material can

8

in this thesis, and in the literature in general, such compounds are referred to as Zintl phases as long as the parent compound is valence-precise.

Figure 1.3: Influence of Zn doping on the room temperature (a) carrier concentration, (b) Seebeck coefficient and conductivity, and (c-d) figure of merit of Ca5In2Sb6.

Figure 1.3 illustrates the effects of doping the Zintl phase Ca5In2Sb6 with an alio-valent element (Zn2+) on the In3+ site. Increasing the Zn content leads to a valence imbalance and thus to increased n (Figure 1.3a), decreased α coefficient and

increased σ (Figure 1.3b), and an improved figure of merit (Figure 1.3 c-d). A single

parabolic band model (SPB model) can be used to approximate the dependence of

σ and α on n (dashed curves in Figure 1.3b) by assuming that the band mass (m∗)

system. While an SPB model can reduce the need to synthesize a large number of samples, the input parameters should ideally be obtained from an extrinsically doped sample, and the model should be employed only at temperatures below the onset of minority carrier effects. A more detailed description of the SPB model and its limitations can be found in ref. [6] and in Chapter 2.

In traditional Zintl phases, the maximum carrier concentration that can be achieved is usually limited by the solubility of the dopant. The chemistry and electronic struc-ture of the Zintl phase also plays a role; doping leads to an electron deficiency in which some bonding states are left unfilled, potentially destabilizing the structure.

Figure 1.4: Left panel: The carrier concentration in Yb14Al1−xMnxSb11 increases

linearly with increasingx. Right panel: In contrast, in Ca5Al2−xMnxSb6,n increases

linearly only at very low Mn concentrations.

Doping Limitations Some Zintl phases are able to tolerate very large dopant

concentrations and show highly degenerate behavior, while in others, doping is very limited. For example, Yb14MSb11 compounds tolerate nH > 1021h+/cm3 [21]. The

Yb14MSb11 structure is valence precise when M is 3+. Yb14MnSb11 (in which Mn is divalent) can thus be regarded as a heavily doped analogue of the valence-precise Zintl phase, Yb14AlSb11. The carrier concentration in the Mn-analogue (nH = 1.2

10

compounds may be partly explained by the presence of several heavy bands (and thus
a large density of states) slightly below the valence band edge [63]. In contrast, the
Ca5Al2Sb6 system tolerates only 5 at% Mn on the Al site, leading to a maximum
carrier concentration of 2 x 1020_{h}+_{/cm}3 _{[64].}

While most Zintl compounds can be doped to obtain degenerate p-type

semi-conducting behavior, n-type behavior is rarely reported. Since n-type doping fills

anti-bonding states in the conduction band, the resulting chemical instability may cause the formation of more stable secondary phases [65]. Alternatively, attempts to increase the Fermi level through n-type chemical doping may encourage the

for-mation of compensating defects (e.g., vacancies, substitutions, or interstitial defects), effectively pinning the Fermi level close to the valence band maximum. In the case ofAZn2Sb2 compounds (A= Ca, Sr, Eu, Yb), this was demonstrated by Pomrehn et

al. [66] using Density Functional theory. The formation enthalpy for cation vacancies was found to decrease with increasing Fermi level, making n-type behavior

thermo-dynamically unattainable due to the inevitable formation of positively charged cation vacancies.

Non-Stoichiometric Phases Stretching the limit of the Zintl formalism are

com-pounds that cannot be synthesized with a valence-precise composition, such as Yb9-Mn4+xSb9. The Yb9Mn4+xSb9 system is valence-precise when x = 0.5. However,

when x is greater than zero, the additional Mn atoms must occupy interstitial sites

[67]. The competing energetic requirements of charge balance and structural stability lead to an electron deficient composition of approximately Yb9Mn4.2Sb9. The

result-ing highp-type carrier concentration (2 x 1020 _{h}+_{/cm}3_{) is very close to the optimal} _{n}
predicted by an SPB model, leading to excellent thermoelectric performance without
the need for doping [68].

Similarly, AZn2Sb2 samples (A = Ca, Sr, Eu, Yb) are consistently found to have

in AZn2Sb2 compounds depend strongly on the electronegativity of A. While

elec-tronegativity influences the degree of electron transfer between the anion and cation in a bond, it does not directly affect the total number of electrons in the valence band or the concentration of free carriers (assuming the valence state of the cation is unaltered). However, the bonding character does influence the bond strength and lattice energy, and, in turn, affects the thermodynamically stable concentration of lattice defects. In this way, the electronegativity of the cation indirectly affects the electronic carrier concentration. This mechanism may be generally applicable, per-haps explaining similar trends seen in A14MnSb11 and A9Mn4+xSb9 (A = Yb or Ca)

based materials [69, 70].

1.3.2

## Band Structure Criteria

When selecting and optimizing Zintl phases for thermoelectric applications, several key characteristics of the electronic band structure should be considered. The most critical requirement is the presence of a band gap (Eg >0), which allows a single

car-rier type to dominate transport. The magnitude of Eg determines the temperature

at which minority carrier effects begin to negatively impact thermoelectric perfor-mance (e.g., bipolar thermal conductivity and degradation of the Seebeck coefficient) [71, 16]. Many Zintl compounds are semiconductors with small band gaps (Eg < 1

eV), although semimetallic Zintl phases, in which the conduction and valence bands overlap (Eg < 0 eV), have also been reported [72]. Good thermoelectric performance

is most often found in materials with band gaps in the range of 0.2 and 0.6 eV. The band mass, anisotropy, and the number of bands involved in transport (band degeneracy, Nv) also play an important role in determining thermoelectric

perfor-mance. The effective mass presents a fundamental conflict; while a light inertial
effec-tive mass (m∗_{i}) along the direction of transport is desired for high mobility (µ=τ /m∗_{i},

whereτ=carrier relaxation time), a heavy “density of states effective mass” (m∗_{DOS}) is

12

improvement in mobility conferred by a light band mass outweighs the detrimental effect on the Seebeck coefficient [73].

The density of states effective mass and the inertial effective mass are related to the band degeneracy by Eq. 1.2. This relationship suggests that when Nv is

large and m∗_{i} is small, a high Seebeck coefficient and high mobility can be obtained

simultaneously [17].

m∗_{DOS} =m∗_{i}N_{v}2/3 (1.2)

Of the Zintl band structures reported to date, the number of bands involved in

p-type transport near the valence band edge varies from one to three. This is far

less than that of the most successful thermoelectric materials such as PbTe and its alloys, which have up to Nv =16 [19]. This disparity is partly explained by the

higher symmetry of the latter compounds, which leads to multiple symmetrically equivalent carrier pockets [17]. However, there is no theoretical limitation on Nv in

Zintl compounds, suggesting that a computational survey may reveal Zintl phases with high Nv.

growing sufficiently large single crystal or oriented polycrystalline samples.

1.3.3

## Carrier Relaxation Time

Figure 1.5: (a) AZn2Sb2 samples (A = Sr, Eu, Ca, Yb) have a broad range of carrier

concentrations, but all can be described by the same band mass (m∗ = 0.6me) within

a single parabolic band model. (b) In contrast, the mobility ofAZn2Sb2 samples varies

widely, suggesting large differences in the carrier relaxation time,τe.

The charge carrier relaxation time, τe, is a critical but often-overlooked transport

parameter. In most bulk thermoelectric materials at high temperature (> 300 K),τ

is limited by acoustic phonon scattering. In this limit, the temperature dependence of the carrier mobility decreases as µH ∝ T−ν, where ν is between 1 and 1.5 for

degenerate and non-degenerate behavior, respectively [76].

The relationship between the magnitude of τe and the structure and chemistry

of Zintl phases is not yet well understood. The AZn2Sb2 series, where A = Sr, Ca,

Eu, or Yb, provides a good example of the large variation in τe that can result from

chemical substitutions. The electronic mobility in AZn2Sb2 compounds is very high

relative to most Zintl phases, in part due to relatively light m∗_{i}. Transport data

suggests that m∗_{DOS} in AZn2Sb2 remains constant regardless of the choice of cation,

as illustrated by the pisarenko curve (Figure 1.5a) generated using an SPB model with an effective mass of m∗ = 0.6 me [75]. Computational studies have also confirmed

14

carrier mobility is found to be significantly higher in the rare earth analogues than in the alkaline earth analogues (Figure 1.5b) [26]. A recent investigation of AZn2Sb2

single crystals (included in Figure 1.5b), by May et. al suggests that this trend is an intrinsic material property, rather than a result of processing [77]. This behavior has not yet been rationalized, and cannot be readily explained by material parameters.

1.4

## Lattice Thermal Conductivity

Reproduced with permission from J. Mater. Chem 21, 15843-15852 (2011).

Copyright © 2011 Royal Society of Chemistry.

1.4.1

Introduction

Thermal conductivity (κ) in bulk semiconductors arises primarily from electronic (κe),

bipolar (κB), and lattice (κL) contributions [78, 79, 80, 7]. The electronic component

is reasonably well-described by the Wiedemann-Franz law, scaling linearly with elec-trical conductivity and temperature according to κe = LT σ. The Lorenz number,

L, can be obtained using classic solutions to the Boltzmann transport equation,

de-scribed in Chapter 2. The bipolar contribution is due to the recombination ofn- and p-type charge carriers on the cool side the sample, releasing energy as heat [71]. This

term is significant only when intrinsic carriers dominate transport (e.g., in compounds with small band gaps, in intrinsic semiconductors, or at very high temperatures). The lattice contribution arises from phonon transport and is the subject of this section.

The discovery of complex, bulk thermoelectric materials with intrinsically low lat-tice thermal conductivity, (e. g., Yb14MnSb11, Ba8Ga16Ge30, XyCo4Sb12) has led to

Figure 1.6: Thermoelectric materials can achieve low lattice thermal conductivity through point scattering sources (Si1−xGex, XyCo4Sb12 [1, 2, 3]), heavy atoms and

anharmonic bonding (PbTe), and complex crystal structures, in which most of the phonon dispersion consists of low velocity optical modes (Yb14MnSb11, Ca3AlSb3, Ba8Ga16Ge30) [4, 5, 6].

scattering and group velocity. Despite these approximations, these models highlight the critical material parameters that ultimately determine thermal conductivity.

To lay the groundwork for a more in-depth examination of factors affecting lattice thermal conductivity, we consider Eq. 1.3, which describes κL as the product of heat

capacity (Cv), phonon velocity (ν), and phonon mean free path (l). This equation

provides a rough guide toκL by neglecting the frequency dependence of each

param-eter. The phonon relaxation time, τ, is related to l by the phonon velocity. The

phonon velocity is often simply approximated by the low frequency speed of sound (νs∝

p

B/d), where B is the appropriate elastic modulus and d is the density of the

material.

κL=

1

3Cvνl = 1 3Cvν

2_{τ} _{(}_{ν} _{=}_{l/τ}_{)} _{(1.3)}

Traditionally, achieving low lattice thermal conductivity has relied on (a) low νs,

found in dense materials with soft bonds, or (b) reduction of τ by the intentional

introduction of point defects and nanostructures to scatter phonons [87, 88, 89, 90, 1, 91]. Figure 1.6 shows the success of these approaches in PbTe and in Si.

While Eq. 1.3 qualitatively describes κL, the universal relaxation time and

16

from experimental results. Crucial to the development of materials with controlled phonon transport is a frequency-dependent description of κL, as all of the terms in

Eq. 1.3 vary significantly across the phonon spectrum. Use of a simplified version of the Callaway model gives Eq. 1.4 [92, 93], which neglects the small correction term for non-resistive (normal) phonon-phonon interactions [79, 81, 82, 94].

κL=

1 3

Z ωmax

0

Cs(ω)νg(ω)2τ(ω)dω (1.4)

The need for frequency-dependent analysis is revealed by considering bulk silicon. Eq. 1.3 yields l = 45 nm at 300 K, using experimentalκL, heat capacity, and speed of

sound. In contrast, a more thorough analysis by Dames et al. using Eq. 1.4 indicates that 80% of the lattice thermal conductivity arises from phonons with mean free paths between 0.1 - 10µm [95]. This latter result is consistent with experimental results

showing significant reduction in κL when phonon scattering sources are induced at

micron length scales [96].

0 π/a

k 0

ω_{D}

Frequency (

ω

) Debye

BvK

ν_{s}

ν_{g}
ν_{p}

Figure 1.7: In a Debye model, the speed of sound (νs), phase velocity (νp), and

group velocity (νg) are equivalent. In contrast, the Born-von Karman model for a

monoatomic chain shows significant curvature of the phonon dispersion.

1.4.2

## Thermal Conductivity within the Debye Model

dω/dk) and phase velocity (νp =ω/k) as the speed of sound,νs (Figure 1.7) [97, 98].

Here, νs is the appropriate average of the longitudinal and transverse velocities at the

low frequency limit. By neglecting the frequency dependence of velocity, we can focus fully on the frequency dependence of the heat capacity and relaxation time. The Debye model has a maximum phonon frequency given by ωmax=ωD = (6π

2

V )

1/3_{ν}

s,

where V is the atomic volume. The corresponding Debye temperature is given by kBΘD =~ωD.

Heat Capacity The Debye specific heat capacity is given by Eq. 1.5. We are

inter-ested in the spectral heat capacity (Cs(ω)), which is the integrand of Eq. 1.5, shown

in Figure 1.8(a) at various temperatures. At high temperature, the frequency de-pendence of Cs(ω) approaches ω2 and can be approximated by Eq. 1.6. Integrating

Eq. 1.6 to ωD yields the Dulong Petit approximation (3kB per atom) for the heat

capacity.

Cv =

3_{~}2
2π2_{k}

BT2 ωmax

Z

0

ω4e~ω/kBT

νgνp2(e~ω/kBT −1)2

dω (1.5)

Cs,HT(ω) =

3kBω2

2π2_{ν}

gνp2

(1.6)

Phonon Relaxation Time The phonon relaxation time, τ(ω), is typically

lim-ited by a combination of phonon-phonon scattering, point defect scattering, and, in nanostructured materials, boundary scattering, which sum according to Eq. 1.7.

τ−1 =X

i

τ_{i}−1 (1.7)

At temperatures above θD, Umklapp phonon-phonon scattering is often the

dom-inant scattering effect. Umklapp scattering depends strongly on the anharmonicity of the bonding, described by the Grüneisen parameter (γ) [99, 100], as well as the

average mass (_{M}¯_{) and temperature (}_{T}_{), as seen in Eq. 1.8. Although many }

expres-sions exist for τU, we emphasize the universality of τU ∝

¯

M ν3

V1/3_{ω}2_{γ}2_{T} and similarity

18

5 10 ω_{D}

0 Frequency (THz) 10-4 10-3 10-2 10-1 1 10

Phonon relaxation time (ns)

0 5 10 ω_{D}

0 Frequency (THz) 0 0.05 0.1 0.15 κ s ( ω )

(pW s m

-1 K

-1 )

0 5 10 ω_{D}

0 Frequency (THz) 0 1 2 3 C v,s ( ω

) (10

-7 J s K

-1 m

-3 ) ∞ 2 1 0.5 0.25 Effective τ Boundary Umklapp PD

Temperature [θ_{D}]

Umklapp

PD Boundary

ω−2

ω2

ω−4

a)

b)

c)

5 10 ω_{D}

0 Frequency (THz) 10-4 10-3 10-2 10-1 1 10

Phonon relaxation time (ns)

0 5 10 ω_{D}

0 Frequency (THz) 0 0.05 0.1 0.15 κ s ( ω )

(pW s m

-1 K

-1 )

0 5 10 ω_{D}

0 Frequency (THz) 0 1 2 3 Cv,s ( ω

) (10

-7 J s K

-1 m

-3 ) ∞ 2 1 0.5 0.25 Effective τ Boundary Umklapp PD

Temperature [θ_{D}]

Umklapp

PD Boundary

ω−2

ω2

ω−4

a)

b)

c)

a) b)

5 10 ω_{D}

0 Frequency (THz) 10-4 10-3 10-2 10-1 1 10

Phonon relaxation time (ns)

0 5 10 ω_{D}

0 Frequency (THz) 0 0.05 0.1 0.15 κ s ( ω )

(pW s m

-1 K

-1 )

0 5 10 ω_{D}

0 Frequency (THz) 0 1 2 3 Cv,s ( ω

) (10

-7 J s K

-1 m

-3 ) ∞ 2 1 0.5 0.25 Effective τ Boundary Umklapp PD

Temperature [θ_{D}]

Umklapp

PD Boundary

ω−2

ω2

ω−4

a)

b)

c)

c)

Figure 1.8: (a) Spectral Debye heat capacity approaches ω2 dependence at high tem-peratures. (b) Frequency dependence of common scattering mechanisms. (c) Top curve: spectral thermal conductivity (assuming νg(ω) = νs and T >> θD) when τU

limits transport. Lower curve: spectral thermal conductivity when τB, and τP D are

also accounted for.

compounds PbTe and PbSe in the context of Eq. 1.8. While heavier, softer PbTe has a lower group velocity than PbSe, the larger Grüneisen parameter of PbSe leads to similarly lowκL [105].

τU(ω) =

(6π2_{)}1/3

2

¯

M νgνp2

kBV1/3γ2ω2T (1.8)

Boundary scattering in polycrystalline materials with grain sizedcan be estimated

SrZnSb2, which was found by transmission electron microscopy to contain numerous stacking faults [108].

τB =

d

νg (1.9)

Scattering by point defects arises from both mass and strain contrast within the lattice. Point defect scattering has been successfully employed in both thermoelectic materials (Si1−xGex), and in thermal barrier coatings such as yttria stabilized zirconia

[1, 91]. Among Zintl materials, this strategy has been very successful in reducingκLin

alloyedAM2Sb2compounds (A= Ca, Eu, Yb, andM = Mn, Zn, Cd) [32, 109, 110, 40] and in Yb9Mn4+xSb9, which contains interstitial Mn [68]. In the simple case of alloying

on a single crystallographic site, τP D is given by Eq. 1.10. Here, fi is the fraction of

atoms with mass mi and radiusri that reside on a site with average mass and radius

¯

m and r¯, respectively [111, 98].

τ_{P D}−1 = V ω

4

4πν2

pνg

X

i

fi

1− mi

¯ m 2 +X i fi 1− ri

¯

r

2

!

(1.10)

The scattering mechanisms discussed above target different populations of phonons, as shown in Figure 1.8b. Umklapp and point defect scattering target high frequency phonons, while boundary scattering is often the dominant scattering mechanism at low frequencies. In concert, these scattering mechanisms lead to an effective τ shown

by the dashed line.

The frequency dependence ofκLcan be used to determine which phonons are

criti-cal to heat transport. The integrand of Eq. 1.4 is commonly referred to as the spectral thermal conductivity,κs(ω) = Cs(ω)νg(ω)2τ(ω). In a defect-free crystal at high

tem-peratures, the ω2 dependence of Cs(ω) is offset by the ω−2 dependence of Umklapp

scattering, resulting in the frequency-independent κs(ω) shown in Fig. 1.8(c).

Inte-grating over the phonon spectrum yields the classic expression forτU-limited κLgiven

in Eq. 1.11 [94, 103].

κU =

(6π2)2/3 4π2

¯

M ν_{s}3

T V2/3_{γ}2 (1.11)

20

and yields reasonable estimates forκLin materials with low mass contrast and simple

crystal structures. In most materials however, boundary and point defect scattering are also significant, resulting in a highly frequency dependent κs(ω). The impact of

boundary and point defect scattering onκLcan be readily visualized as the difference

in area between the top and bottom curves of Fig. 1.8(c).

1.4.3

## Thermal Conductivity in Complex Systems

The following sections consider material systems with phonon dispersions that are progressively more complex than a simple Debye model. Complex phonon dispersions influence κL by (a) changing the states available for Umklapp scattering and (b)

leading to highly frequency-dependent phonon velocities, as νg(ω) =dω/dk [112, 81,

7].

Use of a simple Born-von Kármán (BvK) model allows us to visualize how the crystal structure determines the phonon dispersion. The 1-dimensional BvK model describes the lattice as a chain of atoms connected by springs with harmonic restoring forces [97, 98]. Figure 1.7 compares the Debye and BvK dispersions for the simple case of a monatomic chain [113].

High Mass Contrast The trend between high mass contrast and low lattice

ther-mal conductivity has been clearly demonstrated by Slack [7]. Figure 1.9 reveals that the experimental κL of rock salt compounds is dramatically overestimated by the

Debye model (κU) when mass contrast is high (e. g. BaO, mass ratio of 8.6).

The relationship between mass contrast and κL can be understood by examining

the BvK phonon dispersions for a diatomic chain with varying mass ratio, m1 : m2 (Figure 1.10a). When the mass ratio is low, the Debye model’s assumption of a constant phonon velocity appears reasonable. However, this assumption breaks down as the mass ratio increases and the optical branch flattens [114]. When τ is limited

by Umklapp scattering, the spectral thermal conductivity, κs(ω), is proportional to

νg(ω)2. Figure 1.10b shows the dramatic reduction inνg(ω)2, and thusκL, associated

accounted for here, changes to the phonon dispersion may also influence the available states for scattering events, leading to changes in the spectral mean free paths.

Figure 1.9: Calculated κU (Eq. 1.11) significantly overestimates experimental κL in

rock salt compounds with high mass contrast at T = θD. Values for θD, γ and κL

were obtained from Ref. [7]

a) b)

Figure 1.10: (a) As mass contrast increases in a diatomic chain, (average mass, νs

held constant) the optical mode flattens and the gap increases. (b) The reduction of

κL due to mass contrast can be judged from the area beneath the νg(ω)2 curves.

Complex Primitive Cells Much like the high mass contrast rock-salt compounds,

it has been argued that compounds with a large number of atoms (N) in the primitive

unit cell have low κL due to low velocity optical modes [7, 101]. Classic examples of

high-N compounds with low κL include Y3Al5O12 (N=80), β-Boron (N=105), and

22

Table 1.1: Room temperatureκL in materials with a large number of atoms (N) per

primitive cell.

Material N κL (300 K) Ref.

W/mK

LaPO4 24 2.5 [115]

W3Nb14O44 61 1.8 [115]

LaMgAl11O19 64 1.2 [116]

La2Mo2O9 624 0.7 [115]

α Al14.7Mn3.5Si1.8 138 1.5 [117]

Ca5Al2Sb6 26 1.5 [10]

Ca3AlSb3 28 1.6 [5]

Yb11Sb10 42 0.8 [47]

Yb11In1Sb9 42 0.8 [48]

Yb9Mn4.2Sb9 44 0.5 [68]

Ba8Ga16Ge30 54 1.1 [6, 59]

Yb14AlSb11 104 0.6 [21]

materials for thermoelectrics and thermal barrier coatings (Table 1.1) [4, 115]. To further investigate the trend between low κL and N, we have compiled the

properties of materials for which all of the quantities in Eq. 1.11 are known exper-imentally. Many materials with applications for thermal barrier coatings have not been included, as their Grüneisen parameters are not reported in the literature. We consider the ratio of measured κL to that predicted by κU (Eq. 1.11). Figure 1.11

shows that for simple structures, good agreement between κU and experimental κL

can sometimes be obtained. However,κL of more complex materials are consistently

over-estimated by the simple κU model.

The trend between low κL and structural complexity can be qualitatively

ratio-nalized by a BvK model. Figure 1.12a shows phonon dispersions for 1D chains with

N-atom cells. As N increases, the phonon dispersion “folds in” on itself, resulting in N−1optical modes with lowνg(ω). Thus, in complex materials, the vast majority of

heat is trapped in flat, low velocity optical modes, which are not accurately described by a Debye model. Figure 1.12b emphasizes the reduction of νg(ω)2 (and thus κs(ω)

1 10 100 N

0.01 0.1 1

κ

L/

κ

UN-1/3

N-1

Figure 1.11: For materials with many atoms per primitive cell (N), Eq. 1.11 fails to predict the experimental κL. Data obtained from ref [8].

the lowest experimental lattice thermal conductivities [37].

A promising approach to modeling κLin complex materials, proposed by Toberer

et al. [8], is to consider the acoustic contribution (κa) using a Debye model and the

optical (κo) contribution using Cahill’s model for disordered structures. To determine

the maximum frequency of the acoustic branch, ωa, the equal partition of the heat

capacity amongst the phonon modes (Cv,acoustic =Cv/N) is employed, yielding ωa=

ωD/N1/3 [101]. Values forωa can thus be obtained either from measurements ofνsor

θD. However, the various approaches to obtainingθD (e. g., low or high temperature

heat capacity measurements or density of states from neutron experiments) can yield significantly different values [7, 119].

With ωa determined, the acoustic contribution can be determined from Eq. 1.4

using the high temperature limit for the heat capacity. For τ limited by Umklapp

scattering,κa ∝N−1/3 (Eq. 1.12). If instead, boundary scattering is assumed to

dom-inate transport,κa∝N−1 (Eq. 1.13). In practice, the experimentalN-dependence in

24

0 π/a

k

Frequency (

ω

)

0 π/a

k 0πk/a0kπ/a

Frequency (ω) 0

ν_{s}2

ν g

(

ω

)

2

n = 1 2 4 8

a)

b)

0 π/a

k

Frequency (

ω

)

0 π/a

k 0πk/a0kπ/a

Frequency (ω) 0

ν_{s}2

ν g

(

ω

)

2

n = 1 2 4 8

a)

b)

Figure 1.12: (a) Phonon dispersions for ball and spring chains with increasing number of atoms per unit cell (constantνs). (b) A dramatic decrease inνg(ω)2, and thusκs(ω),

is found with increasing N. For N = 4 and 8, the high frequency optical modes are

not visible on a linear plot due to the extreme flatness of these modes.

Umklapp: κa =

(6π2_{)}2/3

4π2

¯

M ν3

s

T V2/3_{γ}2

1

N1/3

(1.12)

Boundary: κa=

kBνsd

V 1 N (1.13)

Traditional models for κL in materials with complex structures ignore the optical

branches entirely. However, at the amorphous limit (N = ∞), the acoustic contri-bution (κa) approaches zero, whereas in reality, glasses still possess finite thermal

conductivity. For a lower bound to the optical contribution to thermal conductiv-ity (κo), one can look to Einstein’s treatment of heat transport as the diffusion of

heat between atomic oscillators. Cahill has extended this theory to larger oscillating units, for which lglass = λ/2, or equivalently τglass(ω) = π/ω [120, 121]. Note that

lglass =λ/2is still much larger than the average distance between atoms [71]. In this

model, the speed of sound is used to describe the coupling between oscillators. The optical contribution toκLcan thus be estimated by evaluating Eq. 1.4 using τglass, the

κo =

3kBνs

2V2/3

π

6

1/3

(1− 1

N2/3) (1.14)

0.1